Exploration for the Self-ordering of Porous Alumina ... 1 Exploration for the Self-ordering of...
Embed Size (px)
Transcript of Exploration for the Self-ordering of Porous Alumina ... 1 Exploration for the Self-ordering of...
Instructions for use
Title Exploration for the Self-ordering of Porous Alumina Fabricated via Anodizing in Etidronic Acid
Author(s) Takenaga, Akimasa; Kikuchi, Tatsuya; Natsui, Shungo; Suzuki, Ryosuke O.
Citation Electrochimica acta, 211, 515-523https://doi.org/10.1016/j.electacta.2016.06.071
Issue Date 2016-09-02
Doc URL http://hdl.handle.net/2115/71414
Rights © 2016. This manuscript version is made available under the CC-BY-NC-ND 4.0 licensehttp://creativecommons.org/licenses/by-nc-nd/4.0/
Type article (author version)
File Information Etidronic3.pdf
Hokkaido University Collection of Scholarly and Academic Papers : HUSCAP
Exploration for the Self-ordering of Porous Alumina Fabricated via Anodizing in Etidronic Acid Akimasa Takenaga, Tatsuya Kikuchi*,1, Shungo Natsui, and Ryosuke O. Suzuki Faculty of Engineering, Hokkaido University N13-W8, Kita-ku, Sapporo, Hokkaido, 060-8628, Japan *Corresponding author: Tatsuya Kikuchi TEL: +81-11-706-6340 FAX: +81-11-706-6342 E-mail: firstname.lastname@example.org 1 ISE active member
Highlights Etidronic acid anodizing caused self-ordering behaviors between 165 and 270 V. Large-scale pore arrays measuring 470 nm in diameter could be fabricated. Hexagonal phosphorus-free distribution was measured in the porous alumina. A truly honeycomb alumina structure consisting of hexagonal pores was formed.
Abstract Ordered porous alumina (OPA) with large-scale circular and hexagonal pores was fabricated via etidronic acid anodizing. High-purity aluminum plates were anodized in 0.2-4.2 M etidronic acid solution at 145-310 V and 288-323 K. Self-ordering of porous alumina was observed at 165 V and 313 K in 4.2 M, at 205 V and 303 K in 1.0 M, and at 260 V and 298 K in 0.2 M, and the cell diameter was measured to be 400-640 nm. The ordering potential difference decreased with the electrolyte concentration increasing. OPA without an intercrossing nanostructure could be fabricated on a nanostructured aluminum surface via two-step anodizing. Subsequent pore-widening in etidronic acid solution caused the circular dissolution of anodic oxide and the expansion of pore diameters to 470 nm. The shape of the pores was subsequently changed to a hexagon from a circle via long-term pore-widening, and a honeycomb structure with narrow alumina walls and hexagonal pores measuring 590 nm in its long-axis was formed in the porous alumina. Transition of the nanostructure configuration during pore-widening corresponded to differences in the incorporated phosphorus distribution originating from the etidronic acid anions. Keywords: Aluminum; Anodizing; Etidronic Acid; Porous Alumina; Self-Ordering
1. Introduction Anodizing of aluminum and its alloys under appropriate electrochemical conditions allows the formation of ordered porous alumina (OPA) with nanoscale honeycomb structures on aluminum substrates [1-6]. OPA has many nanoscale pores with a high regularity, and can be easily fabricated via a simple anodizing technique without any special equipment or technique such as photolithography, electron-beam lithography, and nanoimprinting (self-ordering). Therefore, it is widely used by many researchers as a template for novel and challenging nanodevices in the fields of electronic and optical applications [7-14]. It is a well-known experimental fact that the periodic size of the OPA, which is called the “cell size” or “interpore distance”, strongly depends on the applied potential difference (voltage) and electrolyte species used for anodizing in the aqueous solutions [2,5,15,16]. Sulfuric acid at an ordering potential difference of 19 V (corresponding cell size: 50 nm) - 25 V (60 nm) [4,5,17-19], oxalic acid at 40 V (100 nm) [4,5,20], selenic acid at 42 V (95 nm) - 48 V (112 nm) [21-23], malonic acid at 120 V (300 nm) , phosphonic acid at 150 V (370 nm) - 180 V (440 nm) , phosphoric acid at 160 V (405 nm) - 195 V (500 nm) [26,27], and tartaric acid at 195 V (500 nm)  have been reported as anodizing electrolytes to date. The bottom shape of the porous alumina exhibits a self-ordered cell structure as a result of rearrangement of the initially disordered cells under the potential difference applied . OPA with large-scale cell sizes and pores is required for expanding the application field in nano- and micro-structure fabrication [28,29]. Recently, we reported an OPA formed via anodizing in the novel electrolyte etidronic acid (1-hydroxyethane-1,1-diphosphonic acid, CH3C(OH)[PO(OH)2]2) . Etidronic acid anodizing at 210-270 V at appropriate temperatures caused the self-ordering behavior of porous alumina, and OPA with large-scale cell diameters of 530-670 nm could be successfully fabricated on aluminum substrates. An ordered aluminum dimple array created from etidronic acid anodizing and subsequent selective oxide dissolution led to a bright structural coloration with a rainbow spectrum due to submicrometer-scale periodic structures. We demonstrated the transfer of the ordered nanostructures to polydimethylsiloxane (PDMS) and ultraviolet (UV) curable polymers via nanoimprinting . In these previous investigations, whole anodizing investigations were carried out in a 0.3 M etidronic acid solution, which is a frequently used electrolyte concentration for anodizing including other electrolyte solutions such as sulfuric, oxalic, and phosphoric acid [17,20,26]. In contrast, we found that anodizing at
different electrolyte concentrations expanded the ordering potential difference and corresponding cell size ranges [22,25]. Therefore, etidronic acid anodizing in various electrolyte concentrations may exhibit undiscovered self-ordering at potential differences over 210-270 V. In the present investigation, we demonstrated etidronic acid anodizing at various electrolyte concentrations and electrochemical operating conditions. OPA with large-scale cell sizes and pore diameters was successfully fabricated via two-step etidronic acid anodizing and subsequent pore-widening. Evaluation and characterization of the OPA, including its nanostructures and elemental distributions, were investigated via high-resolution electron microscopy. A unique honeycomb nanostructure with narrow alumina walls could be fabricated via long-term slow pore-widening and based on the hexagonal distribution of the phosphorus originating from the electrolyte. 2. Experimental High-purity aluminum plates (99.999 wt%, 0.25-1.0 mm thick, GoodFellow, UK) were cut into 10 mm × 20 mm pieces with a handle. The aluminum pieces were ultrasonically degreased in ethanol for 10 min at room temperature. The lower half of the handle of the aluminum specimen was coated with a silicone resin (KE45W, Shin-Etsu, Japan) to avoid the electrochemical reaction on the handle. Prior to silicone resin coating, the aluminum surface on the coated region was mechanically polished with a SiC paper for adhesion improving. After resin coating, the specimens were immersed in a 13.6 M CH3COOH/2.56 M HClO4 (78 vol% CH3COOH/22 vol% 70% HClO4) solution at 280 K and were electropolished at 28 V for 1-10 min. A large aluminum plate (99.99 wt%, Nippon Light Metal, Japan) was used as the cathode, and the solution was slowly stirred with a magnetic stirrer during electropolishing. After electropolishing, the specimens were washed with distilled water and then stored in a drying container. The electropolished specimens were immersed in 0.2-4.2 M etidronic acid solution (150 mL, Tokyo Chemical Industry, Japan) at 288-323 K and then anodized at 145-310 V for up to 24 h using a direct power supply (PWR400H, Kikusui Electronics, Japan) connected to a PC. In the initial stage of anodizing, the potential difference was linearly increased for the first 2.5 min to avoid oxide burning phenomenon as much as possible, and then held at each target potential difference. The inner diameter of the electrochemical cell used for anodizing was 55 mm. A platinum plate (26 mm × 15 mm,
99.95 wt%, Nilaco, Japan) was used as the cathode and was set 15 mm apart from and parallel to the aluminum specimen. The solution was vigorously stirred with a cross-head stir bar. The current density was measured by a digital multimeter (DMM4040, Tektronix, USA) during the anodizing. Details of the anodizing setup have been shown elsewhere  After anodizing, the anodic oxide formed on the aluminum specimens was selectively dissolved in a 0.2 M CrO3/0.51 M H3PO4 solution at 353 K to expose the aluminum substrate. The nanoscale aluminum dimple array corresponding to the negative shape of the bottom of the porous alumina was formed on the aluminum substrate. The extent of the self-ordering behavior was evaluated by fast Fourier transform (FFT). The nanostructured aluminum specimens were anodized again in etidronic acid solution under the same anodizing conditions to fabricate the OPA (two-step anodizing). This process was carried out for the formation of OPA with whole vertical regions. After the two-step anodizing, the specimens were immersed in a 1.0 M etidronic acid solution at 298 K for up to 72 h to expand the diameter of the pores in the OPA (pore-widening). The aluminum specimens in each step were examined by field emission scanning electron microscopy (FE-SEM, JSM-6500F and JIB-4600F/HKD, JEOL, Japan). For the observation of anodic oxide, a thin platinum